Output from "TOTOPOL", (version 1.92, 17 Jul 2017, Mike Treacy).

Report for the framework in file "public/tmp/tmp_225_6_76714_mYrveL.cif"

There are 1152 T-atoms per unit cell
There are 2304 O-atoms per unit cell

Framework density = 13.05 T-atoms per nm^3
Material density = 1.302 grams per cm^3 (excluding extra-framework material)
-------------------------------------------------------------------
-------------------------- T-O Analysis ---------------------------
-------------------------------------------------------------------
[Si] Ideal SiO distance = 1.610 Angstrom
T1  -- O1  = 1.6184 Angstrom
T1  -- O2  = 1.6174 Angstrom
T1  -- O3  = 1.6957 Angstrom
T1  -- O4  = 1.7041 Angstrom
      mean = 1.6589 Angstrom
        t1 = 0.044911  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.021449  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T2  -- O3  = 1.6826 Angstrom
T2  -- O5  = 1.6574 Angstrom
T2  -- O6  = 1.6410 Angstrom
T2  -- O7  = 1.6016 Angstrom
      mean = 1.6457 Angstrom
        t1 = 0.035866  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.020234  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T3  -- O4  = 1.6383 Angstrom
T3  -- O8  = 1.6930 Angstrom
T3  -- O9  = 1.4593 Angstrom
T3  -- O10 = 1.7112 Angstrom
      mean = 1.6254 Angstrom
        t1 = 0.097965  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.107323  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T4  -- O7  = 1.5450 Angstrom
T4  -- O9  = 1.4573 Angstrom
T4  -- O11 = 1.6147 Angstrom
T4  -- O12 = 1.6091 Angstrom
      mean = 1.5565 Angstrom
        t1 = 0.065648  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.036705  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T5  -- O10 = 1.7367 Angstrom
T5  -- O13 = 1.6847 Angstrom
T5  -- O14 = 1.6240 Angstrom
T5  -- O15 = 1.6003 Angstrom
      mean = 1.6614 Angstrom
        t1 = 0.057638  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.030030  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T6  -- O12 = 1.6325 Angstrom
T6  -- O15 = 1.6117 Angstrom
T6  -- O16 = 1.6163 Angstrom
T6  -- O17 = 1.6131 Angstrom
      mean = 1.6184 Angstrom
        t1 = 0.009810  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.005503  (0.0 is a perfect tetrahedron)

        T-O SUMMARY
          Range  = 1.4573 A <--> 1.7367 A
          Mean   = 1.6277 A
          StdDev = 0.0671 A

       t1 Range  = 0.0098 <-- 0.0520 --> 0.0980
       t2 Range  = 0.0055 <-- 0.0369 --> 0.1073

-------------------------------------------------------------------
------------------------- O-T-O Analysis --------------------------
-------------------------------------------------------------------
O1  -- T1  -- O2  = 107.623 deg; O1  -- O2  = 3 A
O1  -- T1  -- O3  = 108.002 deg; O1  -- O3  = 3 A
O1  -- T1  -- O4  = 107.781 deg; O1  -- O4  = 3 A
O2  -- T1  -- O3  = 108.051 deg; O2  -- O3  = 3 A
O2  -- T1  -- O4  = 108.297 deg; O2  -- O4  = 3 A
O3  -- T1  -- O4  = 116.759 deg; O3  -- O4  = 3 A
       107.623 deg <-- 109.419 deg --> 116.759 deg

O3  -- T2  -- O5  = 114.263 deg; O3  -- O5  = 3 A
O3  -- T2  -- O6  = 110.248 deg; O3  -- O6  = 3 A
O3  -- T2  -- O7  = 107.062 deg; O3  -- O7  = 3 A
O5  -- T2  -- O6  = 112.019 deg; O5  -- O6  = 3 A
O5  -- T2  -- O7  = 105.976 deg; O5  -- O7  = 3 A
O6  -- T2  -- O7  = 106.780 deg; O6  -- O7  = 3 A
       105.976 deg <-- 109.391 deg --> 114.263 deg

O4  -- T3  -- O8  = 113.219 deg; O4  -- O8  = 3 A
O4  -- T3  -- O9  =  94.008 deg; O4  -- O9  = 2 A
O4  -- T3  -- O10 = 117.402 deg; O4  -- O10 = 3 A
O8  -- T3  -- O9  = 109.799 deg; O8  -- O9  = 3 A
O8  -- T3  -- O10 = 120.877 deg; O8  -- O10 = 3 A
O9  -- T3  -- O10 =  95.304 deg; O9  -- O10 = 2 A
       94.008 deg <-- 108.435 deg --> 120.877 deg

O7  -- T4  -- O9  =  98.216 deg; O7  -- O9  = 2 A
O7  -- T4  -- O11 = 107.570 deg; O7  -- O11 = 3 A
O7  -- T4  -- O12 = 117.859 deg; O7  -- O12 = 3 A
O9  -- T4  -- O11 = 114.167 deg; O9  -- O11 = 3 A
O9  -- T4  -- O12 = 105.779 deg; O9  -- O12 = 2 A
O11 -- T4  -- O12 = 112.606 deg; O11 -- O12 = 3 A
       98.216 deg <-- 109.366 deg --> 117.859 deg

O10 -- T5  -- O13 = 121.559 deg; O10 -- O13 = 3 A
O10 -- T5  -- O14 = 107.855 deg; O10 -- O14 = 3 A
O10 -- T5  -- O15 = 104.788 deg; O10 -- O15 = 3 A
O13 -- T5  -- O14 = 107.718 deg; O13 -- O14 = 3 A
O13 -- T5  -- O15 = 106.358 deg; O13 -- O15 = 3 A
O14 -- T5  -- O15 = 107.899 deg; O14 -- O15 = 3 A
       104.788 deg <-- 109.363 deg --> 121.559 deg

O12 -- T6  -- O15 = 111.913 deg; O12 -- O15 = 3 A
O12 -- T6  -- O16 = 108.449 deg; O12 -- O16 = 3 A
O12 -- T6  -- O17 = 109.291 deg; O12 -- O17 = 3 A
O15 -- T6  -- O16 = 108.486 deg; O15 -- O16 = 3 A
O15 -- T6  -- O17 = 109.288 deg; O15 -- O17 = 3 A
O16 -- T6  -- O17 = 109.377 deg; O16 -- O17 = 3 A
       108.449 deg <-- 109.467 deg --> 111.913 deg

        O-T-O SUMMARY
          Range  = 94.0081 deg <--> 121.5586 deg
          Mean   = 109.2435 deg
          StdDev = 5.9391 deg

        O--O SUMMARY
          Range  = 2.2689 A <--> 2.9861 A
          Mean   = 2.6525 A
          StdDev = 0.1563 A

-------------------------------------------------------------------
------------------------- T-T-T Analysis --------------------------
-------------------------------------------------------------------
-------------------------------------------------------------------
------------------------- T-O-T Analysis --------------------------
-------------------------------------------------------------------
T1  -- O1  -- T1  = 143.373 deg ; T1  -- T1   3.0729 A

T1  -- O2  -- T1  = 156.942 deg ; T1  -- T1   3.1696 A

T1  -- O3  -- T2  = 142.242 deg ; T1  -- T2   3.1966 A

T1  -- O4  -- T3  = 123.617 deg ; T1  -- T3   2.9461 A

T2  -- O5  -- T2  = 127.954 deg ; T2  -- T2   2.9788 A

T2  -- O6  -- T2  = 125.883 deg ; T2  -- T2   2.9228 A

T2  -- O7  -- T4  = 129.659 deg ; T2  -- T4   2.8478 A

T3  -- O8  -- T3  = 144.380 deg ; T3  -- T3   3.2237 A

T3  -- O9  -- T4  = 143.043 deg ; T3  -- T4   2.7662 A

T3  -- O10 -- T5  = 146.335 deg ; T3  -- T5   3.3001 A

T4  -- O11 -- T4  = 100.170 deg ; T4  -- T4   2.4770 A

T4  -- O12 -- T6  = 148.820 deg ; T4  -- T6   3.1223 A

T5  -- O13 -- T5  = 132.179 deg ; T5  -- T5   3.0802 A

T5  -- O14 -- T5  = 142.869 deg ; T5  -- T5   3.0789 A

T5  -- O15 -- T6  = 128.719 deg ; T5  -- T6   2.8957 A

T6  -- O16 -- T6  = 114.296 deg ; T6  -- T6   2.7156 A

T6  -- O17 -- T6  = 115.227 deg ; T6  -- T6   2.7244 A


        T-O-T SUMMARY
          Range  = 100.1695° <--> 156.9417 deg
          Mean   = 133.2768 deg
          StdDev = 14.2657 deg

        T--T SUMMARY
          Range  = 2.4770 A <--> 3.3001 A
          Mean   = 2.9717 A
          StdDev = 0.2108 A

-------------------------------------------------------------------
------------------------ *** WARNINGS *** -------------------------
-------------------------------------------------------------------

SOME OXYGEN ATOMS ARE TOO CLOSE TO EACH OTHER
O4  -- O9  = 2.2689 A
O7  -- O9  = 2.2702 A

T-T-T analysis was not conducted.
T3  -- T4  = 2.7662 Angstrom

SOME T-ATOM DISTANCES ARE OUTSIDE THE NORMAL RANGE
T4  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T4  -- T2  = 2.8478 Angstrom
  T4  -- T3  = 2.7662 Angstrom
  T4  -- T4  = 2.4770 Angstrom
  T4  -- T5  = 3.4966 Angstrom
  T4  -- T6  = 3.1223 Angstrom
T5  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T5  -- T3  = 3.3001 Angstrom
  T5  -- T4  = 3.4966 Angstrom
  T5  -- T5  = 3.0802 Angstrom
  T5  -- T5  = 3.0789 Angstrom
  T5  -- T6  = 2.8957 Angstrom
T6  -- T6  = 2.7156 Angstrom
T6  -- T6  = 2.7244 Angstrom

-------------------------------------------------------------------
---------------------- Topological Analysis -----------------------
-------------------------------------------------------------------
T1 (Si): multiplicity = 192
Coordination Sequence =
    1 4 9 18 30 43 60 78 96 120 149 184 227 269 308 351 397
TD10 = 608
Circuit symbol = 4.8.4.8.4.10_{5}
Weight = 22
Vertex symbol  = 4.8.4.8.4.12
Weight = 27

T2 (Si): multiplicity = 192
Coordination Sequence =
    1 4 9 15 22 32 48 72 99 125 150 175 204 240 286 339 390
TD10 = 577
Circuit symbol = 4.4.4.6.6.6_{4}
Weight = 15
Vertex symbol  = 4.4.4.6.6_{3}.8_{2}
Weight = 23

T3 (Si): multiplicity = 192
Coordination Sequence =
    1 4 9 15 25 40 54 70 92 119 152 187 222 264 312 354 391
TD10 = 581
Circuit symbol = 4.4.4.6_{2}.6.6_{5}
Weight = 12
Vertex symbol  = 4.4.4.6_{2}.6_{4}.8
Weight = 16

T4 (Si): multiplicity = 192
Coordination Sequence =
    1 4 8 12 17 27 44 65 88 113 144 182 219 249 278 319 372
TD10 = 523
Circuit symbol = 4.4.4.4.6_{3}.6_{4}
Weight = 14
Vertex symbol  = 4.4.4.4.6.6_{2}
Weight = 14

T5 (Si): multiplicity = 192
Coordination Sequence =
    1 4 9 16 24 35 51 72 101 131 157 190 228 262 301 351 406
TD10 = 601
Circuit symbol = 4.4.4.8_{3}.6.6_{3}
Weight = 10
Vertex symbol  = 4.4.4.12_{5}.6_{2}.12_{4}
Weight = 32

T6 (Si): multiplicity = 192
Coordination Sequence =
    1 4 9 14 19 28 43 63 86 115 151 190 228 262 293 324 364
TD10 = 533
Circuit symbol = 4.6.4.6_{2}.4.6_{3}
Weight = 16
Vertex symbol  = 4.6.4.6_{2}.4.6_{3}
Weight = 16

<TD10> = 570.500
Average ring size = 5.6652
